Fabrication and Processing of Metal Alloys (L-II) Dr.RabiulHussain School of Material Science & Engineering Jimma Institute of Technolgy, Jimma University E-mail: firstname.lastname@example.org Ph.No. +251-0966882081 (Ethiopia) +91-9508832510 (India
Fabrication & Processing of metal alloys • What are the common fabrication techniques for metals? • How do the properties vary throughout a piece of metal that has been quenched? • How can properties be modified by a post heat treatment?
Fabrication of Metals Fabrication: Metal fabrication is the building of metal structures by cutting, bending, and assembling processes. It is a value added process that involves the construction of machines and structures from various raw materials. • Metal fabrication techniques are normally preceded by refining, alloying, and often heat-treating processes that produce alloys with the desired characteristics. • Fabrication techniques depend on many factors: • properties of metal • the size and the shape of the finished piece • cost
Fabrication of Metals • Metal fabrication techniques are mainly four kinds: • Casting: give a shape by pouring in liquid metal into a mold that holds the required shape, and letting harden the metal without external pressure. • Forming–to give shape in solid state by applying pressure. • Machining–in which material is removed in order to give it the required shape. • Joining–where different part are joined by various means. • Other important technique is powder metallurgy.
Metal Casting • Pouring molten metal into a mold cavity having the desired shape. • This technique is employed when: • product is large and/or complicated shape • particular material is low in ductility. • More economical
SAND CASTING • The common casting method where sand is used as casting material. A two piece mold (cope and drag) is formed by compact packing of sand around a pattern of required shape. An addition gating is provided for proper distribution of liquid metal. • AdvantagesThis process can be used for a large range of sizes and for small or large production runs. It is the cheapest casting process available for small production runs and can sometimes be economical for large production runs.
Die Casting • Here metal is forced into mold by external pressure at high velocities. Usually a permanent two-piece mold made of steel is used. In this technique rapid cooling rates are achieved, thus inexpensive.
INVESTMENT CASTING • In this pattern is made of wax. Then fluid slurry of casting material is poured over which eventually hardens and holds the required shape. Subsequently, pattern material is heated to leave behind the cavity. • This technique is employed when high dimensional accuracy, reproduction of fine details, and an excellent finish are required.
Continuous Casting • After refining metals are usually in molten state, which are later solidified into ingots for further processing like forming. In continuous casting, solidification and primary forming process are combined, where refined metal is cast directly into a continuous strand which is cooled by water jets. This technique is highly automated and more efficient. Uniform composition through-out the casting is achievable when compared with ingot-cast products.
Metal Forming Operations • Forming operations are those in which the shape of a metal piece is changed by plastic deformation. • The deformation must be induced by an external force or stress, the magnitude of which must exceed the yield strength of the material • These are basically two types – one that performed at relatively low temperatures, cold working; ad the other performed at high temperatures, hot working.
Hot Working • When deformation is achieved at a temperature above that at which recrystallization occurs, the process is termed hot working. • Advantages of Hot Working: • Lower forces and power than in cold working • More intricate work geometries possible • Need for annealing may be reduced or eliminated • Capability for substantial plastic deformation of the metal - far more than possible with cold working or hot working • Why? – Strength coefficient is substantially less than at room temp. – Strain hardening exponent is zero (theoretically) – Ductility is significantly increased
Cold Working • Performed at room temperature or slightly above. • Many cold forming processes are important mass production operations. • Minimum or no machining usually required – These operations are near net shape or net shape processes. Advantages of Cold Forming vs. Hot Working: • Better accuracy, closer tolerances • Better surface finish • Strain hardening increases strength and hardness • Grain flow during deformation can cause desirable directional properties in product • No heating of work required (less total energy)
Rolling • Rolling, the most widely used deformation process, consists of passing a piece of metal between two rolls; a reduction in thickness results from compressive stresses exerted by the rolls. • Deformation is terms of reduction in thickness resulting from applied compressive forces. • This technique is typically employed to produce sheets, strips, foil, I-beams, rails, etc. Fig. Rolling
Forming Processes: Forging • This involves deforming a single piece of metal, usually, by successive blows or continuous squeezing. • In open die forging, two dies having same shape is employed, usually, over large work-pieces. • In closed die forging, there may be more than two pieces of die put together having finished shape. • Forged products have outstanding grain structures and very good mechanical properties. Fig. Closed die Forging
Drawing • It is pulling of material though die orifice using tensile forces. Again a reduction in cross-section results with corresponding change in length. Drawing die entrance is at angle against to extrusion die which is usually rectangular. • Typical drawing strand includes number of dies in a series sequence. • Rods, wire, and tubes are commonly produced using drawing technique. Fig. Drawing
Extrusion • For extrusion, a bar of metal is forced through a die orifice by a compressive force that is applied to a ram; the extruded piece that emerges has the desired shape and a reduced cross-sectional area. • Typical extrusion products are: rods, (seamless) tubes, complicated shapes for domestic purpose. Fig. EXTRUSION
Machining • This technique employs removable of metal from selected areas of the workpiece to give final shape to the product. This is in direct contrast with metal forming where metal is moved and volume is conserved. • Machining usually is employed to produce shapes with high dimensional tolerance, good surface finish, and often with complex geometry. • When number of product pieces required is small, machining is preferred over forming as special tool cost will be less.
JOINING • There been many joining techniques, especially for metallic materials. These include: welding, brazing, soldering, and riveting. • In these techniques, two pieces are joined together either by adhesive/cohesive bonding and/or mechanical locking. • Welding, brazing, and soldering involve melting of either parent metal or external metallic liquid (filler material) which upon cooling provides cohesive bonds. • In riveting, pieces are put together by mechanical locking. These techniques are employed to join two pieces of same metal with complicated shapes, or of different metals because of difficulty in fabricating them using one of the previous methods. • This may be employed when on-part fabrication is expensive or inconvenient.
WELDING • In welding, two or more metal parts are joined to form a single piece when one part fabrication is expensive or inconvenient. Both similar and dissimilar metals may be welded. • The joining bond is metallurgical (involving some diffusion) rather than just mechanical as with riveting and bolting. • Different welding methods include : ARC AND GAS WELDING, BRAZING, SOLDERING, LASER BEAM WELDING. • During arc and gas welding, the workpieces to be joined and the filler material (i.e.,welding rod) are heated to a sufficiently high temperature to cause both to melt; upon solidification, the filler material forms a fusion joint between the workpieces. Thus,there is a region adjacent to the weld that may have experienced microstructural and property alterations; this region is termed the heat-affected zone
WELDING Fig: Cross sectional representation showing the zones in the vicinity of a typical Fusion weld
pressure heat area contact densify densification point contact by diffusion at at low T higher T POWDER METALLURGY This method involves: • Blending fine powdered materials, • pressing them into a desired shape or form (compacting), and then • heating the compressed material in a controlled atmosphere to bond the material (sintering). • Metals having high melting temperatures are difficult to melt and cast, and the fabrication is expedited using P/M. Rhodium metal: powder, pressed pellet (3×105 psi), remelted
THERMAL PROCESSING • Two main kinds of metal processing methods–mechanical and thermal. • Thermal processing is also known as heat treatment. • Purpose of heat treatment: -improvement in ductility -relieving internal stresses -grain size refinement -increase of strength -improvement in machinability and toughness • Thermal processing factors–temperature up to which material is heated, length of time that the material is held at the elevated temperature, rate of cooling, and the surrounding atmosphere under the thermal treatment.
Thermal Processing Methods • Two kinds heat treating methods are–annealing and quenching & tempering. • These differ in the way material is cooled from an elevated temperature. • Annealing involves cooling the material slowly, allowing phase changes. • Quenching (also known as hardening) means cooling the material at a rapid rate to arrest the equilibrium phase transformations. • During annealing ,material is cooled in air and /or heating furnace itself. • For quenching, material is immersed in water/oil quench bath.
Annealing Processes • Annealing can be defined as a heat treatment process in which the material is taken to a high temperature, kept there for some time and then slowly cooled. • High temperatures allow diffusion processes to occur fast. The time at the high temperature (soaking time) must be long enough to allow the desired transformation to occur. • Cooling is done slowly to avoid the distortion (warping) of the metal piece, or even cracking, caused by stresses induced by differential contraction due to thermal inhomogeneities. • Benefits of annealing are: • relieve stresses • increase softness, ductility and toughness • produce a specific microstructure
Types of Annealing Process • Process annealing–appliedto cold worked materials to negate effects of cold work. During this heat treatment, material becomes soft and thus its ductility will be increased considerably. Commonly sandwiched between two cold work operations. Improves ductility. • Stress relief operation removes the stresses that might have been generated during plastic deformation, non-uniform cooling, or phase transformation. Unless removed, these stresses may cause distortion of components. Temperature used is normally low such that effects resulting from cold working are not affected.
Types of Annealing Process • Full annealing is normally used for products that are to be machined subsequently, such as transmission gear blanks. After heating and keeping at an elevated temperature, components are cooled in furnace to effect very slow cooling rates. Typically, the product receives additional heat treatments after machining to restore hardness and strength . • Normalizing is used to refine the grains and produce a more uniform and desirable size distribution. It involves heating the component to attain single phase (e.g.: austenite in steels), then cooling in open air atmosphere.
Thermal Processing of Metals • Stress Relief: Reduce • Spheroidize (steels): stress caused by: Make very soft steels for -plastic deformation good machining. Heat just -nonuniform cooling below TE & hold for -phase transform. 15-25h. • Full Anneal (steels): Types of Make soft steels for Annealing good forming by heating g to get , then cool in furnace to get coarse P. • Process Anneal: Negate effect of • Normalize (steels): cold working by Deform steel with large (recovery/ grains, then normalize recrystallization) to make grains small. Annealing: Heat to Tanneal, then cool slowly. Based on discussion in Section 11.7, Callister 7e.
QUENCING AND TEMPERING PROCESS • Quenching is heat treatment process where material is cooled at a rapid rate from elevated temperature to produce Martensite phase. This process is also known as hardening. Rapid cooling rates are accomplished by immersing the components in a quench bath that usually contains quench media in form of either water or oil, accompanied by stirring mechanism. • Quenching operation is usually followed by tempering. • Tempering involves heating martensitic steel at a temperature below the eutectoid transformation temperature to make it softer and more ductile. Here Martensite transforms to ferrite embedded with carbide particles.
QUENCHING AND TEMPERING • Martempering is a modified quenching procedure used to minimize distortion and cracking that may develop during uneven cooling of the heat-treated material. It involves cooling the austenized steel to temperature just above Ms temperature, holding it there until temperature is uniform, followed by cooling at a moderate rate to room temperature before austenite-to-bainite transformation begins. The final structure of martempered steel is tempered Martensite. • Austempering is different from martempering in the sense that it involves austenite-to-bainite transformation. Thus, the structure of austempered steel is bainite. • Advantages of austempering are – improved ductility; decreased distortion and disadvantages are – need for special molten bath; process can be applied to limited number of steels.
Case Hardening • In case hardening, the surface of the steel is made hard and wear resistant, but the core remains soft and tough. Such a combination of properties is desired in applications such as gears. • INDUCTION HARDENING: Here, an alternating current of high frequency passes through an induction coil enclosing the steel part to be heat treated. The induced emf heats the steel. In induction hardening, the heating time is usually a few seconds. Immediately after heating, water jets are activated to quench the surface. Martensite is produced at the surface, making it hard and wear resistant. The microstructure of the core remains unaltered.
Case Hardening II. Flame Hardening: For large work pieces and complicated cross-sections induction heating is not easy to apply. In such cases, flame hardening is done by means of an oxyacetylene torch. Heating should be done rapidly by the torch and the surface quenched, before appreciable heat transfer to the core occurs.
Case Hardening Laser Beam Hardening: In this case, a laser beam can be used for surface hardening. As laser beams are of high intensity, a lens is used to reduce the intensity by producing a defocused spot of size ranging from 0.5 to 25 mm. Proper control of energy input is necessary to avoid melting. Laser hardening has the advantage of precise control over the area to be hardened, an ability to harden reentrant surfaces, very high speed of hardening and no separate quenching step.
Case hardening techniques • Carburizing is the most widely used method of surface hardening. Here, the surface layers of low carbon steel are enriched with carbon up to 0.8-1.0%. The source of carbon may be a solid medium, a liquid or a gas. In all cases, the carbon enters the steel at the surface and diffuses into the steel as a function of time at an elevated temperature. Carburizing is done at 920-950o C. • Two methods:
Case Hardening Techniques • Cyaniding is done in a liquid bath of NaCN, with the concentration varying between 30 and 97%. The temperature used for cyaniding is lower than that for carburizing and is in the range of 800-870o C. The time of cyaniding is 1-3 hr to produce a case depth of 0.25 mm or less. • Nitriding is carried out in the ferritic region. No phase change occurs after nitriding. The part to be nitrided should posses the required core properties prior to nitriding. During nitriding, pure ammonia decomposes to yield nitrogen which enters the steel. The solubility of nitrogen in ferrite is small. Most of the nitrogen, that enters the steel, forms hard nitrides (e.g., Fe3N). The temperature of nitriding is 500-590o C. The time for a case depth of 0.02 mm is about 2 hr. In addition to providing outstanding wear resistance, the nitride layer increases the resistance of carbon steel to corrosion in moist atmospheres.
THANK YOU FOR ATTENTION